- Email: [email protected]

Contents lists available at ScienceDirect

Thin Solid Films j o u r n a l h o m e p a g e : w w w. e l s ev i e r. c o m / l o c a t e / t s f

Effective optical properties of highly ordered mesoporous thin ﬁlms Neal J. Hutchinson, Thomas Coquil, Ashcon Navid, Laurent Pilon ⁎ University of California, Los Angeles, Henry Samueli School of Engineering and Applied Science, Mechanical and Aerospace Engineering Department, 420 Westwood Plaza, Los Angeles, CA 90095-1597, USA

a r t i c l e

i n f o

Article history: Received 22 March 2009 Received in revised form 11 August 2009 Accepted 31 August 2009 Available online 9 September 2009 Keywords: Mesoporous Optical materials Photocatalysis Coatings Optoelectronics devices Dielectric constant Effective medium approximation

a b s t r a c t This paper expands our previous numerical studies predicting the optical properties of highly ordered mesoporous thin ﬁlms from two-dimensional (2D) nanostructures with cylindrical pores to threedimensional (3D) structures with spherical pores. Simple, face centered, and body centered cubic lattices of spherical pores and hexagonal lattice of cylindrical pores were considered along with various pore diameters and porosities. The transmittance and reﬂectance were numerically computed by solving 3D Maxwell's equations for transverse electric and transverse magnetic polarized waves normally incident on the mesoporous thin ﬁlms. The effective optical properties of the ﬁlms were determined by an inverse method. Reﬂectance of 3D cubic mesoporous thin ﬁlms was found to be independent of polarization, pore diameter, and ﬁlm morphology and depended only on ﬁlm thickness and porosity. By contrast, reﬂectance of 2D hexagonal mesoporous ﬁlms with cylindrical pores depended on pore shape and polarization. The unpolarized reﬂectance of 2D hexagonal mesoporous ﬁlms with cylindrical pores was identical to that of 3D cubic mesoporous ﬁlms with the same porosity and thickness. The effective refractive and absorption indices of 3D ﬁlms show good agreement with predictions by the 3D Maxwell–Garnett and nonsymmetric Bruggeman effective medium approximations, respectively. © 2009 Elsevier B.V. All rights reserved.

1. Introduction Mesoporous thin ﬁlms have been studied extensively in recent years [1–7]. Potential applications include dye-sensitized solar cells [8–10], low-k dielectric materials [11,12], photocatalysis [13,14], biosensors [15–17], optoelectronics [18–20], and antireﬂecting and self-cleaning coatings [21], to name a few. In these applications, predicting the effects of porosity and pore shape, size, and spatial arrangement on the optical and dielectric properties is essential to the design of mesoporous materials with desired performances or for material characterization purposes. Signiﬁcant progress has been made in synthesizing mesoporous thin ﬁlms with various morphologies as well as pore shapes and sizes using evaporation induced self-assembly of micelles in polymer precursors [1–6]. Highly ordered mesoporous materials made of dielectrics (e.g., SiO2, [1–5]) or semi-conductors (e.g., TiO2 [3], Si [6], Ge, Ge/Si alloys [7]) have been synthesized in the form of ﬁlms, ﬁbers, and/or powders [1]. The choices of surfactant (e.g., Cetyl trimethylammonium bromide, Pluronics, Brij) and of the initial alcohol/water/ surfactant mole fractions determine the size and shape of the pores as well as the ﬁnal mesostructure [1]. For example, P63/mmc space group structure featuring spherical pores arranged in 3D compact hexagonal packing, Pm3n space group structure with spherical pores in compact cubic arrangement, and p6m space group structure where ⁎ Corresponding author. Tel.: +1 310 206 5598; fax: +1 310 206 2302. E-mail address: [email protected] (L. Pilon). 0040-6090/$ – see front matter © 2009 Elsevier B.V. All rights reserved. doi:10.1016/j.tsf.2009.08.048

cylindrical pores arranged in 2D compact hexagonal lattice have been synthesized [1–5]. The dielectric and optical constants of the mesoporous materials can then be tailored by controlling the porosity [22,23] or by introducing optically active materials within the pores [14,21]. Various effective medium approximations (EMAs) have been proposed to predict the dielectric and/or optical properties of heterogeneous nanocomposite thin ﬁlms by treating them as homogeneous media with some effective refraction and absorption indices denoted by neff and keff, respectively [24]. The most commonly used EMAs are the Maxwell–Garnett theory (MGT) [24,25], Drude [26,27] (also called the Silberstein formula [24,28]), symmetric and nonsymmetric Bruggeman [24,29], Lorentz–Lorenz [26,30–32], parallel [33] (also called Birchak formula [24]) and Volume Averaging Theory (VAT) [34,35] models. Expressions for these models are summarized in Table 1. The MGT model is expressed for both 3D spherical inclusions (3D MGT) and 2D cylindrical inclusions (2D MGT) [24]. In brief, the effective properties (subscript “eff”) are expressed as functions of the porosity and the properties of the continuous phase (subscript “c”) and of the dispersed phase (subscript “d”). However, these EMAs are independent of polarization, pore size, shape, or spatial arrangement. Note that the VAT model is identical to the Drude model when continuous and dispersed phases are non-absorbing, i.e., kc = kd = 0.0. Most models have been developed for the effective dielectric constant or refraction index but not for the absorption index. Given the multitude of models one may wonder which one to use and the choice has often been arbitrary. Others may wish to achieve further tuning of

2142

N.J. Hutchinson et al. / Thin Solid Films 518 (2010) 2141–2146

Table 1 Expressions of different effective medium approximations (EMAs) widely used in the literature. EMA model 3D Maxwell–Garnett Theory (3D MGT) 2D Maxwell–Garnett Theory (2D MGT) Drude (or Silberstein) Symmetric Bruggeman

Formula

Ref.

n2eff

= n2c 1−

n2eff

= n2c 1−

2fv ðn2c −n2d Þ

[24]

n2c + n2d + fv ðn2c −n2d Þ

n2eff = ð1−fv Þn2c + fv n2d ð1−fv Þ

n2c −n2eff n2c + 2n2eff

+ fv

n2d + 2n2eff

eff − d 2 2

n n 1−fv = " 1c= 3 c

n2eff −1 n2eff + 2

=0

[24,29]

n2 d n2 c

#

[24]

1−

= ð1−fv Þ

[26,27]

n2d −n2eff

n2

n2 eff n2 c

Lorentz–Lorenz

[25]

2n2c + n2d + fv ðn2c −n2d Þ

n 2 Nonsymmetric Bruggeman

3fv ðn2c −n2d Þ

n2c −1

n2c + 2

+ fv

n2d −1

n2d + 2

[31,32,43]

A = fv ðn2d −k2d Þ + ð1−fv Þðn2c −k2c Þ Volume Averaging Theory (VAT)

B = 2nd kd fv + 2nc kc ð1−fv Þ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 n2eff = ½A + A2 + B2 2 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 k2eff = ½−A + A2 + B2 2

Parallel (or Birchak)

neff = ð1−fv Þnc + fv nd

[34,35]

[24]

the effective dielectric and optical properties by controlling the pore size and the ﬁlm morphology. This study aims to address both of these questions. It was enabled by advances in computational methods and parallel computing as well as ever greater available computer resources. Previous studies [36–38] established that reﬂectance and effective optical properties of two-dimensional mesoporous thin ﬁlms with cylindrical pores exposed to normally incident transverse electric (TE) and transverse magnetic (TM) waves depended on electromagnetic (EM) wave polarization. For TE polarization, the pore shape and size had no effect on the effective optical properties which were predicted by the VAT model [36,37]. For TM polarization, the parallel model was in good agreement with the retrieved effective optical properties for pores with cylindrical cross-section [38]. In addition, pore shape and spatial arrangement had a strong effect on the retrieved effective properties. The present study extends our previous investigations of 2D nonabsorbing [36] and absorbing nanocomposite ﬁlms with cylindrical pores [37,38] to 3D absorbing mesoporous thin ﬁlms with spherical pores. Three-dimensional Maxwell's equations were solved numerically to compute the transmittance and reﬂectance over the spectral range of 400 to 900 nm. The numerical results were compared with predictions from the different EMAs and with results previously reported [38].

Fig. 1. Schematic of the 3D physical model of simple cubic mesoporous thin ﬁlms simulated with fv = 6.5% and L/D = 6.0.

(TM) polarizations are deﬁned such that the incident electric and magnetic ﬁeld vectors are parallel to the cylindrical pores main axis, respectively. In other words, the incident electric ﬁeld vector is such → → that E 0 = E0 → e z for TE polarization and E 0 = E0→ e y for TM polarization as illustrated in Fig. 1. The ﬁgure shows a physical model of a simple cubic mesoporous thin ﬁlm with three spherical pores of diameter D = 5 nm, ﬁlm thickness L = 30 nm, and lattice side length dk = 10 nm. For this morphology, the porosity is expressed as fv = πD3 / 6d3k = 6.54%. Three-dimensional time-harmonic TE and TM polarized electromagnetic plane waves propagating through space have timedependent electric and magnetic ﬁelds expressed as, → → → → iωt Eðx; y; z; tÞ = ½Ex ðx; y; z; tÞ ex + Ey ðx; y; z; tÞ ey + Ez ðx; y; z; tÞ ez e

ð1Þ

2. Analysis

→ → → → iωt Hðx; y; z; tÞ = ½Hx ðx; y; z; tÞ ex + Hy ðx; y; z; tÞ ey + Hz ðx; y; z; tÞ ez e ð2Þ

2.1. Governing equations and numerical implementation

→ → where H is the magnetic ﬁeld, E is the electric ﬁeld, while → e x, → e y and → ez are unit vectors in the Cartesian coordinate system, and ω = 2πc0 / λ is the angular frequency of the EM wave of wavelength λ in vacuum. → → Electric and magnetic ﬁelds E and H satisfy the 3D wave equations for general time-varying ﬁelds given by [39],

The cubic mesoporous thin ﬁlms simulated consisted of a continuous solid matrix with embedded spherical pores. They were deposited on a non-absorbing substrate (medium 3, m3 = n3 − ik3 = n3 − i0.0) and surrounded by a vacuum (medium 1, m1 = 1.0 − i0.0) where mj = nj − ikj is the complex index of refraction of medium “j” and nj and kj are the refraction and absorption indices, respectively. All interfaces were assumed to be optically smooth. Linearly polarized TE or TM plane waves were normally incident to the top surface of the mesoporous thin ﬁlms. Here, transverse electric (TE) and magnetic

→ → → 1 2 ∇ × Eðx; y; z; tÞ −ω εr ε0 Eðx; y; z; tÞ = 0 μμ r 0 → 1 → → 2 ∇× ∇ × Hðx; y; z; tÞ −ω μr μ0 Hðx; y; z; tÞ = 0 εr ε0

∇×

ð3Þ ð4Þ

N.J. Hutchinson et al. / Thin Solid Films 518 (2010) 2141–2146

where ε0 and μ0 are the dielectric permittivity and the magnetic permeability of vacuum, respectively while μr is the relative magnetic permeability of the medium, and εr = m2 = n2 − k2 − i2nk is its complex dielectric constant. Maxwell's equations for TE and TM polarized waves traveling in heterogeneous structures are subject to the boundary conditions provided in Table 2 [39]. The energy ﬂux of the EM wave corresponds to the magnitude of → → the Poynting vector → π , deﬁned as, → π = E × H [40]. The time→ + ye → + ze → averaged averaged Poynting vector at location → r = xe x y z → → → 1 over the period 2π / ω is given by j → π j = Ref E × H*g where H⁎ is 2 → the complex conjugate of vector H [40]. The ﬁlm transmittance is deﬁned as Tnum = |πx,t|avg / |πx,0|avg where |πx,t|avg is the x-component of the time-averaged transmitted Poynting vector further averaged over the ﬁlm–substrate interface while |πx,0|avg is the x-component of the time-averaged incident Poynting vector averaged over the ﬁlm–vacuum interface. Similarly, the reﬂectance is deﬁned as Rnum = |πx,r|avg / |πx,0|avg where |πx,r|avg is the x-component of the time-averaged reﬂected Poynting vector averaged over the ﬁlm–vacuum interface. COMSOL Multiphysics 3.4 was used to numerically solve the 3D Maxwell's equations and the associated boundary conditions using the Galerkin ﬁnite element method on unstructured meshes and using parallel computing on a Dell Precision 690 with two 2.33 GHz QuadCore Intel Xeon CPU and 24 GB of RAM. Transmittance and reﬂectance were computed for 40 wavelengths between 400 and 900 nm. The numerical results were determined to be converged by increasing the number of ﬁnite element meshes by a factor of 1.3 until the maximum relative error in reﬂectance and transmittance between two consecutive mesh reﬁnements was less than 3% and 1%, respectively. A total of 65,310 and 16,472 tetrahedral elements were necessary to obtain a converged solution for cubic and hexagonal mesoporous ﬁlms, respectively. The average relative differences in reﬂectance and transmittance between two consecutive mesh reﬁnements for all wavelengths were less than 1.2% and 0.47%, respectively. This resulted in a maximum relative difference for neff and keff between two mesh reﬁnements of less than 0.73% and 0.71%, respectively.

2143

Expressions for Tth (λi) and Rth (λi) are well-known and can be found in Eqs. (18)–(20) in Ref. [38] and need not be repeated. The effective index of refraction neff and absorption index keff that minimize δT +δR were determined using the generalized reduced gradient nonlinear optimization method [41]. Treating mesoporous thin ﬁlms as homogeneous rests upon the assumption that EM wave scattering by the pores is negligible which prevails when the size parameter 2πD /λ is much smaller than unity [40]. For all simulations reported in this study, the xcomponent of the local time-averaged transmitted Poynting vector |πx,t| was nearly uniform and always within 0.1% of its surface-averaged value |πx,t|avg. Furthermore, the magnitudes of the y- and z-components of the time-averaged Poynting vector averaged over the ﬁlm–substrate interface were found to be negligible compared with |πx,t|avg. Indeed, the maximum values of the ratios |πy,t|avg / |πx,t|avg and |πz,t|avg / |πx,t|avg were less than 2.3 × 10− 3 and 1.1× 10− 3, respectively for all simulations. Thus, scattering the EM wave by the pores was found to be negligible and the mesoporous ﬁlms could be treated as homogeneous with some effective optical properties. 2.3. Validation of the numerical procedure and retrieval method In order to validate the numerical procedure predicting reﬂectance and transmittance as well as the retrieval method for neff and keff, an absorbing dense ﬁlm (Medium 2) with known properties was simulated. The ﬁlm was 600 nm thick and its refraction and absorption indices were assumed to be constant and equal to n2 = 1.44 and k2 = 0.01. It was deposited on a non-absorbing substrate with index of refraction n3 = 3.39. The medium above the dense ﬁlm was a vacuum (n1 = 1.0 and k1 = 0.0). The numerical transmittance and reﬂectance were calculated for TE and TM polarized incident waves. The maximum relative error between the numerical and theoretical transmittance and reﬂectance for TE and TM polarization was 0.012% and 0.011%, respectively. The retrieved complex index of refraction was m 2 = 1.44 − i0.0099 for TE polarization and m2 = 1.4339 − i0.0099 for TM polarization instead of the input value of m2 = 1.44 − i0.01. This difference is small and acceptable. Therefore, the 3D numerical simulation tools used to determine the spectral transmittance and reﬂectance as well as the inverse method to retrieve the ﬁlm complex index of refraction were validated and were used for cubic and hexagonal mesoporous thin ﬁlms.

2.2. Retrieval of effective complex index of refraction The effective refraction and absorption indices neff and keff of the mesoporous thin ﬁlm were retrieved from numerically computed reﬂectance and transmittance by minimizing the root mean square of the relative error for transmittance δT and reﬂectance δR expressed as,

3. Results and discussion

1 N T ðλ Þ−Tnum ðλi Þ 2 1 N Rth ðλi Þ−Rnum ðλi Þ 2 2 2 δT = ∑ th i and δR = ∑ N i=1 Tth ðλi Þ N i=1 Rth ðλi Þ

3.1. Effect of pore diameter and ﬁlm thickness

ð5Þ

The effect of polarization, ﬁlm thickness, and pore diameter was investigated by modeling absorbing simple cubic mesoporous thin ﬁlms consisting of continuous and dispersed phases such that mc = 1.4 − i0.01 and md = m1 = 1.0 − i0.0. The ﬁlm substrate was such that m3 = 3.39 − i0.0. Two values of pore diameter D were tested

where Tth (λi) and Rth (λi) correspond to EM wave theory predictions at N = 40 different incident wavelengths λi treating the mesoporous ﬁlm as homogeneous with some effective optical properties neff and keff.

Table 2 Boundary conditions associated with Maxwell's equations for TE and TM polarizations [39]. Boundary Source surface

TE polarization →

→

TM polarization →

→

→

Dispersed-continuous phase interface

→

→

→

rﬃﬃﬃﬃﬃﬃﬃﬃﬃ μr μ0 → Ez = 0 εr ε0 →

→

→

→

→

→

→

→

rﬃﬃﬃﬃﬃﬃﬃﬃﬃ μr μ0 → Hz = 0 εr ε0

→

→

n × ðE1 −E2 Þ = 0

→

→

→

→

n × E = 0 at boundaries normal to E0

→

→

→

−n × E +

n × ðH 1 − H 2 Þ = 0

→

Symmetry boundaries

→

n×H+

→

n × ð∇ × EÞ−i ωn c0 n × ð E × n Þ = rﬃﬃﬃﬃﬃﬃﬃﬃﬃ i →→ μr μ0 → h → → → → −i k; r n × ð k × H 0 Þ × i ωn c0 ð n− k Þ e εr ε0

h→ i →→ → → → −i k; r − n × E0 × i ωn c0 ð n− k Þ e

Film–substrate interface

→

→

n × ð∇ × E Þ−i ωn c0 n × ðE × n Þ =

n × H = 0 at boundaries normal to H 0

→

→

→

→

→

→

n × E = 0 at boundaries normal to E0

→

→

n × H = 0 at boundaries normal to H 0

2144

N.J. Hutchinson et al. / Thin Solid Films 518 (2010) 2141–2146

embedded in the effective medium itself [24,29]. The Lorentz–Lorenz model was developed for sets of spherical particles in air [31,32]. However, as previously discussed, these models have been used for the index of refraction of various composite materials regardless of the validity of the assumptions for which they had been developed. In other words they have often been chosen arbitrarily and used extensively as discussed in details in [42]. In order to assess the validity of the different EMAs for 3D mesoporous thin ﬁlms, the continuous phase complex index of refraction was chosen as mc = 4.0 − i0.01 while md = m1 = 1.0 − i0.0 and m3 = 3.39 − i0.0 over the spectral range from 400 to 900 nm. These values were chosen to ensure large enough differences between EMAs and were yet realistic. Fig. 3 compares the retrieved effective refraction and absorption indices for the simulated mesoporous ﬁlms with the different EMAs listed in Table 1 for porosity ranging from 0 to 50%. It shows the previously obtained results for TE and TM polarizations on 2D mesoporous ﬁlms with cylindrical pores [38] and the results for 3D ﬁlms with spherical pores arranged in simple cubic mesostructure. It is evident that the retrieved neff and keff decreased as porosity increased. As previously reported, both neff and keff for 2D mesoporous ﬁlms are accurately predicted by the VAT model for TE polarization [36,37]. For TM polarization however, neff is accurately predicted by the 2D MGT model while keff is better predicted by the parallel model [38]. On the contrary, the same values

Fig. 2. Evolution of the retrieved effective refraction and absorption indices of mesoporous thin ﬁlms for TE and TM polarizations as a function of L/D for fv = 9.76% and D = 2 or 50 nm.

namely 2 and 50 nm. The ﬁlm thickness L was varied so that the L/D ratio ranged from 10 to 250. A numerically converged solution was obtained with 33,000 to 100,000 tetrahedral elements for L/D ratio ranging from 10 to 250. Fig. 2 plots the evolution of the retrieved effective refraction and absorption indices neff and keff for TE and TM polarizations as a function of L/D for mesoporous thin ﬁlms with porosity of 9.76%. However, for L/D ≥ 150, the relative difference in neff and keff between pore diameters of 2 and 50 nm and TE and TM polarization was less than 0.03% and 0.57%, respectively. In other words, the effective refraction and absorption indices of the 3D simple cubic ﬁlms were independent of polarization, ﬁlm thickness, and pore diameter for L/ D ≥ 150. This is consistent with results reported by Braun and Pilon [36] for TE polarized waves on 2D ﬁlms with cylindrical pores. Thus, all mesoporous thin ﬁlms simulated in the remaining of this study were such that L/D ≥ 150. 3.2. Effective medium approximations for TE and TM waves Most of the EMAs summarized in Table 1 have been developed for the effective dielectric constant with speciﬁc arrangements. For instance, the MGT model was derived for randomly organized spherical inclusions and small volume fractions [24,25]. The Bruggeman model treats both phases identically as each spherical inclusion is

Fig. 3. Effective refraction and absorption indices as a function of porosity for 2D and 3D simple cubic ﬁlms exposed to normally incident TE and TM polarized waves and having mc = 4.0 − i0.01 and md = 1.0 − i0.0 over the spectral range of 400 to 900 nm.

N.J. Hutchinson et al. / Thin Solid Films 518 (2010) 2141–2146

2145

of neff and keff were retrieved for TE and TM polarized wave incident on 3D mesoporous ﬁlms. Indeed, the maximum relative errors for neff and keff between TE and TM polarizations were 0.52% and 0.71%, respectively. This result was expected by virtue of the fact that the material is isotropic so that TE and TM polarizations which can be deﬁned numerically, are physically equivalent or undeﬁned. However, this gives further conﬁdence in the proper implementation of the numerical simulations as well as in the reported results. For 3D cubic mesoporous ﬁlms, the numerical results for the effective index of refraction neff agrees with the 3D MGT model with a maximum relative error of 1.86%. Note that this was expected since the 3D MGT model was speciﬁcally derived for spherical inclusions and small volume fractions. On the other hand, results for the effective absorption index keff were best approximated by the nonsymmetric Bruggeman model with a maximum relative error of 0.57%. Although no EMA was derived for the effective absorption index keff this information is of interest from a practical point of view. Finally, these results conﬁrm that EMAs for neff and keff should not be chosen arbitrarily.

3.3. Effect of morphologies

Fig. 5. Reﬂectance as a function of wavelength for 300 nm thick mesoporous ﬁlms with fv = 30% and simple cubic, FCC, BCC, and hexagonal morphologies (see Figs. 1 and 4). The pore diameter was adjusted to preserve the same porosity for all ﬁlms.

According to the EMAs listed in Table 1, the effective optical properties depend only on porosity and are independent of polarization, and pore size, shape, and spatial arrangement. However, these assumptions were found to be erroneous for 2D mesoporous ﬁlms with cylindrical pores [38]. This was also investigated in the present study for 3D ﬁlms. To do so, mesoporous thin ﬁlms with simple cubic, body centered cubic (BCC), and face centered cubic (FCC) arrangements with spherical pores, along with hexagonal arrangements with cylindrical pores (see Fig. 4) were numerically simulated. For all morphologies the porosity was set to be 30%, the ﬁlm thickness was 300 nm, and mc = 1.44 − i0.0 while md = m1 = 1.0 − i0.0 and m3 = 3.39 − i0.0. The pore diameter was adjusted to keep the porosity identical for all ﬁlms and was equal to 4.16 nm for

simple cubic, 3.30 nm for BCC, 2.60 nm for FCC, and 2.88 nm for hexagonal. Fig. 5 shows the computed reﬂectance for simple cubic, BCC, and FCC mesoporous ﬁlms with spherical pores and that for hexagonal mesoporous ﬁlm with cylindrical pores. Due to their symmetric morphology, the reﬂectance of simple cubic, BCC, and FCC mesoporous ﬁlms was found to be independent of polarization. Fig. 5 indicates that the reﬂectance of cubic mesoporous ﬁlms was independent of pore size and morphology. On the contrary, the computed reﬂectance from hexagonal mesoporous thin ﬁlms was different for TE and TM polarizations [38]. The reﬂectance of the different cubic mesoporous thin ﬁlms with spherical pores fell between that of the hexagonal

Fig. 4. Schematic of numerically simulated morphologies identical to those of body centered cubic (BCC), face centered cubic (FCC), and hexagonal synthesized mesoporous thin ﬁlms. Simple cubic morphology is shown in Fig. 1.

2146

N.J. Hutchinson et al. / Thin Solid Films 518 (2010) 2141–2146

mesoporous ﬁlm with cylindrical pores for TE and TM polarizations. The reﬂectance of the hexagonal ﬁlm exposed to unpolarized incident light corresponds to the arithmetic mean of the reﬂectance for TE and TM polarizations. It was found to be nearly identical to that of simple cubic, BCC, and FCC mesoporous ﬁlms. The maximum relative differences in neff and keff for the different morphologies were 0.3% and 3.3%, respectively. These results establish that the effective optical properties of 3D structures with spherical pores are only dependent on porosity as assumed by the EMAs. Finally, actual mesoporous silica ﬁlms are open nanostructure featuring interconnected pores. However, the interconnection does not contribute signiﬁcantly to the overall ﬁlm porosity and therefore the above conclusions also apply to actual ﬁlms as validated with experimental data by Hutchinson et al. [42]. 4. Conclusion This study expanded our previous studies for 2D mesoporous ﬁlms with cylindrical pores [36–38] by numerically simulating mesoporous ﬁlms in 3D with spherical pores exposed to TE and TM polarized incident waves. 3D Maxwell's equations were numerically solved to compute the transmittance and reﬂectance of the mesoporous thin ﬁlms over the spectral range from 400 to 900 nm. The effective optical properties of the simple cubic ﬁlms were found to be independent of morphology, polarization, pore size, and ﬁlm thickness for L/D ≥ 150 and depended only on porosity. This study also established that the size, and spatial arrangement (simple cubic, BCC, or FCC) of the spherical pores have no effect on the reﬂectance or the effective refraction and absorption indices of mesoporous thin ﬁlms of identical porosity. Finally, the 3D MGT and the nonsymmetric Bruggeman should be used to predict the refractive and absorption indices of 3D cubic mesoporous thin ﬁlms with spherical pores, respectively. References [1] C.J. Brinker, Y. Lu, A. Sellinger, H. Fan, Adv. Mater. 11 (7) (1999) 579. [2] H. Fan, H.R. Bentley, K.R. Kathan, P. Clem, Y. Lu, C.J. Brinker, J. Non-Cryst. Solids 285 (1–3) (2001) 79. [3] P.C.A. Alberius, K.L. Frindell, R.C. Hayward, E.J. Kramer, G.D. Stucky, B.F. Chmelka, Chem. Mater. 14 (2002) 3284. [4] B.W. Eggiman, M.P. Tate, H.W. Hillhouse, Chem. Mater. 18 (2006) 723. [5] D. Grosso, F. Cagnol, G.J. de A.A. Soler-Illia, E.L. Crepaldi, H. Amenitsch, A. BrunetBruneau, A. Bourgeois, C. Sanchez, Adv. Funct. Mater. 14 (4) (2004) 309. [6] E.K. Richman, C.B. Kang, T. Brezesinski, S.H. Tolbert, Nano Lett. 8 (9) (2008) 3075. [7] D. Sun, A.E. Riley, A.J. Cadby, E.K. Richman, S.D. Korlann, S.H. Tolbert, Nature 441 (7097) (2006) 1126. [8] B. O'Regan, M. Grätzel, Nature 353 (1991) 737. [9] P. Ravirajan, S.A. Haque, D. Poplavskyy, J.R. Durrant, D.D.C. Bradley, J. Nelson, Thin Solid Films 451–452 (2004) 624. [10] L. Schmidt-Mende, M. Grätzel, Thin Solid Films 500 (1–2) (2006) 296. [11] M.I. Sanchez, J.L. Hedrick, T.P. Russell, J. Polym. Sci., B, Polym. Phys. 33 (2) (1995) 253. [12] M.I. Sanchez, J.L. Hedrick, T.P. Russell, Microporous and Macroporous Materials Materials Research Society Symposium Proceedings, vol. 431, Materials Research Society, Pittsburgh, PA, 1996, p. 475. [13] Q. Hu, R. Kou, J. Pang, T.L. Ward, M. Cai, Z. Yang, Y. Lu, J. Tang, Chem. Commun. (2007) 601. [14] D.G. Shchukin, D.V. Sviridovy, J. Photochem. Photobiol., C Photochem. Rev. 7 (1) (2006) 23. [15] M. Arroyo-Hernandez, R.J. Martin-Palma, J. Perez-Rigueiro, J.P. Garcia-Ruiz, J.L. Garcia-Fierro, J.M. Martinez-Duart, Mater. Sci. Eng. C 23 (6–8) (2003) 697. [16] R.J. Martin-Palma, V. Torres-Costa, M. Arroyo-Hernandez, M. Manso, J. PerrezRigueiro, J.M. Martinez-Duart, Microelectron. J. 35 (1) (2004) 45. [17] S. Chan, Y. Li, L.J. Rothberg, B.L. Miller, P.M. Fauchet, Mater. Sci. Eng. C 15 (1–2) (2001) 277. [18] A. Loni, L.T. Canham, M.G. Berger, R. Arens-Fischer, H. Munder, H. Luth, H.F. Arrand, T.M. Benson, Thin Solid Films 276 (1–2) (1996) 143. [19] H.F. Arrand, T.M. Benson, A. Loni, R. Arens-Fischer, M.G. Krueger, M. Thoenissen, H. Lueth, S. Kershaw, N.N. Vorozov, J. Lumin. 80 (1–4) (1998) 119. [20] A. Jain, S. Rogojevic, S. Ponoth, N. Agarwal, I. Matthew, W.N. Gill, P. Persans, M. Tomozawa, J.L. Plawsky, E. Simonyi, Thin Solid Films 398–399 (2001) 513. [21] A.L. Penard, T. Gacoin, J.P. Boilot, Acc. Chem. Res. 40 (9) (2007) 895. [22] A.R. Balkenede, F.K. de Theije, J.C.K. Kriege, Adv. Mater. 15 (2) (2003) 139. [23] C. Jin, S. Lin, J.T. Wetzel, J. Electron. Mater. 30 (4) (2001) 284.

[24] A. Sihvola, Electromagnetic Mixing Formulas and Applications, IEE Electromagnetic Waves Series, vol. 47, The Institution of Electrical Engineers, London, UK, 1999. [25] J.C. Maxwell-Garnett, Philos. Trans. R. Soc. Lond., A 203 (359–371) (1904) 385. [26] N.K. Sahoo, S. Thakur, R.B. Tokas, N.M. Kamble, Appl. Surf. Sci. 253 (16) (2007) 6787. [27] C.-C. Lee, C.-J. Tang, Appl. Optics 45 (36) (2006) 9125. [28] L. Silberstein, Ann. Phys. Chem., Leipzig (1895) 661. [29] D.A.G. Bruggeman, Ann. Phys. 416 (7 and 8) (1935) 636 665. [30] S. Bosch, J. Ferr-Borrull, J. Sancho-Parramon, Solid-State Electron. 45 (5) (2001) 703. [31] L. Lorenz, Ann. Phys. Chem. 247 (9) (1880) 70. [32] H.A. Lorentz, Ann. Phys. Chem. 245 (4) (1880) 641. [33] D.J. Taylor, P.F. Fleig, S.L. Hietala, Thin Solid Films 332 (1–2) (1998) 257. [34] J.A. del Rio, S. Whitaker, Transp. Porous Media 39 (2) (2000) 159. [35] J.A. del Rio, S. Whitaker, Transp. Porous Media 39 (3) (2000) 259. [36] M.M Braun, L. Pilon, Thin Solid Films 496 (2006) 504. [37] A. Garahan, L. Pilon, J. Yin, I. Saxena, J. Appl. Phys. 101 (1) (2007) 014320. [38] A. Navid, L. Pilon, Thin Solid Films 516 (12) (2008) 4159. [39] J. Jin, The Finite Element Method in Electromagnetics, Wiley Press, New York, NY, 2002. [40] M.F. Modest, Radiative Heat Transfer, Academic Press, San Diego, CA, 2003. [41] L.S. Lasdon, A.D. Waren, A. Jain, M. Ratner, ACM Trans. Math. Softw. 4 (1) (1978) 34. [42] N. Hutchinson, T. Coquil, E.K. Richman, S.H. Tolbert, L. Pilon, Reﬂectance of surfactant templated mesoporous silica thin ﬁlms: simulations versus experiments, Thin Solid Films (this issue). [43] D.E. Aspnes, Am. J. Phys. 50 (8) (1982) 704.

Nomenclature c: speed of light [m/s] dk: lattice side length [nm] D: pore diameter [nm] → E: electric ﬁeld vector [V/m] → ex, → e ,→ e : unit vectors of Cartesian coordinate system → y z H: magnetic ﬁeld vector [A/m] k: absorption index → k: wavevector [m− 1] L: thickness of the mesoporous thin ﬁlm [nm] m: complex index of refraction, p = n − ik n: refractive index → n: normal vector to surface of interest N: number of wavelengths considered → r : position vector (r→ =→ ex +→ ey +→ ez) [m] R: reﬂectance T: transmittance t: time [s] x, y, z: spatial coordinates [m]

Greek symbols ε0: permittivity of free space (= 8.85 × 10− 12 F/m) ε′,r εr″: real and imaginary parts of ε*r εr: complex dielectric constant, εr = m2 = εr′ − iεr″ fv: porosity λ: wavelength [nm] μ0: magnetic permeability of free space (=4π × 10− 7 H/m) μr: relative permeability, μr = μ / μ0 → π: Poynting vector [W/m2] |→ π |: time-averaged Poynting vector [W/m2] σ: electrical conductivity [1/Ω m] ω: angular frequency [rad/s]

Subscripts 0: refers to vacuum, or an incident wave 1: refers to surroundings in thin ﬁlm system 2: refers to thin ﬁlm 3: refers to substrate avg: refers to surface-averaged value c: refers to continuous phase d: refers to dispersed phase eff: refers to effective property i: refers to summation index num: refers to numerical result r: refers to reﬂected Poynting vector th: refers to theoretical calculation (see Ref. [38]) t: refers to transmitted Poynting vector x: refers to x-component y: refers to y-component z: refers to z-component